#------------------------------------------------------------------------------
#$Date: 2019-10-07 09:55:39 +0300 (Mon, 07 Oct 2019) $
#$Revision: 219116 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/43/7234398.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7234398
loop_
_publ_author_name
'Alessia Provino'
'Simon Steinberg'
'Volodymyr Smetana'
'Ruta Kulkarni'
'Sudesh K. Dhar'
'Pietro Manfrinetti'
'Anja-Verena Mudring'
_publ_section_title
;
 Gold-rich R3Au7Sn3: establishing the interdependence between electronic
 features and physical properties
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              8311
_journal_page_last               8321
_journal_paper_doi               10.1039/C5TC00884K
_journal_volume                  3
_journal_year                    2015
_chemical_formula_sum            'Au7 Sn3 Y3'
_chemical_formula_weight         2001.57
_space_group_IT_number           176
_space_group_name_Hall           '-P 6c'
_space_group_name_H-M_alt        'P 63/m'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   8.1480(12)
_cell_length_b                   8.1480(12)
_cell_length_c                   9.3940(19)
_cell_measurement_reflns_used    3357
_cell_measurement_temperature    293(2)
_cell_volume                     540.11(16)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_measurement_method       w-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0607
_diffrn_reflns_av_sigmaI/netI    0.0373
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            3357
_diffrn_reflns_theta_full        27.49
_diffrn_reflns_theta_max         27.49
_diffrn_reflns_theta_min         2.17
_exptl_absorpt_coefficient_mu    117.283
_exptl_absorpt_correction_T_max  0.25
_exptl_absorpt_correction_T_min  0.18
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    12.307
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregular fragment'
_exptl_crystal_F_000             1640
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.06
_refine_diff_density_max         2.294
_refine_diff_density_min         -3.547
_refine_diff_density_rms         0.562
_refine_ls_extinction_coef       0.00032(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.049
_refine_ls_matrix_type           full
_refine_ls_number_parameters     25
_refine_ls_number_reflns         439
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.049
_refine_ls_R_factor_all          0.0455
_refine_ls_R_factor_gt           0.0295
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0227P)²+4.7152P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0597
_refine_ls_wR_factor_ref         0.0645
_reflns_number_gt                346
_reflns_number_total             439
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            J-Mater-Chem-C-2015-3-8311.cif
_cod_data_source_block           Y3Au7Sn3
_cod_original_sg_symbol_H-M      P63/m
_cod_database_code               7234398
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Au1 Au 0.34814(11) 0.32994(12) 0.09548(7) 0.0112(2) Uani 1 1 d . . .
Au2 Au 0.6667 0.3333 0.2500 0.0099(4) Uani 1 6 d S . .
Y3 Y 0.6703(4) 0.6938(4) 0.2500 0.0117(5) Uani 1 2 d S . .
Sn5 Sn 0.3333 0.6667 0.0432(2) 0.0066(5) Uani 1 3 d S . .
Sn6 Sn 0.0000 0.0000 0.0000 0.0191(8) Uani 1 6 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Au Au -2.0133 8.8022 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Sn5 Au1 Sn5 112.53(3) . 7_665
Sn5 Au1 Au1 99.92(4) . 10_556
Sn5 Au1 Au1 116.78(4) 7_665 10_556
Sn5 Au1 Sn6 110.23(3) . .
Sn5 Au1 Sn6 109.02(3) 7_665 .
Au1 Au1 Sn6 107.969(14) 10_556 .
Sn5 Au1 Au2 122.30(3) . .
Sn5 Au1 Au2 56.13(4) 7_665 .
Au1 Au1 Au2 60.652(14) 10_556 .
Sn6 Au1 Au2 127.24(3) . .
Sn5 Au1 Y3 67.92(5) . 3_565
Sn5 Au1 Y3 177.97(5) 7_665 3_565
Au1 Au1 Y3 61.23(3) 10_556 3_565
Sn6 Au1 Y3 72.43(5) . 3_565
Au2 Au1 Y3 121.88(3) . 3_565
Sn5 Au1 Y3 160.24(5) . 2_655
Sn5 Au1 Y3 84.32(5) 7_665 2_655
Au1 Au1 Y3 61.96(3) 10_556 2_655
Sn6 Au1 Y3 71.38(5) . 2_655
Au2 Au1 Y3 57.73(5) . 2_655
Y3 Au1 Y3 94.88(9) 3_565 2_655
Sn5 Au1 Y3 65.87(5) . .
Sn5 Au1 Y3 82.97(5) 7_665 .
Au1 Au1 Y3 62.68(3) 10_556 .
Sn6 Au1 Y3 167.70(4) . .
Au2 Au1 Y3 56.89(5) . .
Y3 Au1 Y3 95.52(8) 3_565 .
Y3 Au1 Y3 108.15(7) 2_655 .
Sn5 Au1 Au1 56.91(3) . 7_665
Sn5 Au1 Au1 55.62(2) 7_665 7_665
Au1 Au1 Au1 124.24(3) 10_556 7_665
Sn6 Au1 Au1 127.20(4) . 7_665
Au2 Au1 Au1 88.39(3) . 7_665
Y3 Au1 Au1 124.79(6) 3_565 7_665
Y3 Au1 Au1 138.69(5) 2_655 7_665
Y3 Au1 Au1 61.56(4) . 7_665
Sn5 Au1 Y3 82.09(6) . 7_665
Sn5 Au1 Y3 64.22(6) 7_665 7_665
Au1 Au1 Y3 176.90(5) 10_556 7_665
Sn6 Au1 Y3 69.04(5) . 7_665
Au2 Au1 Y3 120.27(5) . 7_665
Y3 Au1 Y3 117.79(6) 3_565 7_665
Y3 Au1 Y3 115.69(6) 2_655 7_665
Y3 Au1 Y3 120.40(3) . 7_665
Au1 Au1 Y3 58.84(5) 7_665 7_665
Sn5 Au1 Au1 136.87(5) . 8
Sn5 Au1 Au1 54.34(3) 7_665 8
Au1 Au1 Au1 122.97(2) 10_556 8
Sn6 Au1 Au1 55.465(7) . 8
Au2 Au1 Au1 86.38(2) . 8
Y3 Au1 Au1 126.82(5) 3_565 8
Y3 Au1 Au1 61.10(3) 2_655 8
Y3 Au1 Au1 135.69(5) . 8
Au1 Au1 Au1 97.08(4) 7_665 8
Y3 Au1 Au1 54.86(5) 7_665 8
Sn5 Au2 Sn5 180.0 4_665 7_665
Sn5 Au2 Y3 90.0 4_665 3_665
Sn5 Au2 Y3 90.0 7_665 3_665
Sn5 Au2 Y3 90.0 4_665 2_655
Sn5 Au2 Y3 90.0 7_665 2_655
Y3 Au2 Y3 120.0 3_665 2_655
Sn5 Au2 Y3 90.0 4_665 .
Sn5 Au2 Y3 90.0 7_665 .
Y3 Au2 Y3 120.0 3_665 .
Y3 Au2 Y3 120.0 2_655 .
Sn5 Au2 Au1 119.348(14) 4_665 2_655
Sn5 Au2 Au1 60.652(14) 7_665 2_655
Y3 Au2 Au1 63.30(5) 3_665 2_655
Y3 Au2 Au1 65.03(5) 2_655 2_655
Y3 Au2 Au1 150.635(15) . 2_655
Sn5 Au2 Au1 60.652(14) 4_665 11_656
Sn5 Au2 Au1 119.348(14) 7_665 11_656
Y3 Au2 Au1 63.30(5) 3_665 11_656
Y3 Au2 Au1 65.03(5) 2_655 11_656
Y3 Au2 Au1 150.635(15) . 11_656
Au1 Au2 Au1 58.70(3) 2_655 11_656
Sn5 Au2 Au1 60.652(14) 4_665 12_666
Sn5 Au2 Au1 119.348(15) 7_665 12_666
Y3 Au2 Au1 65.03(5) 3_665 12_666
Y3 Au2 Au1 150.635(15) 2_655 12_666
Y3 Au2 Au1 63.30(5) . 12_666
Au1 Au2 Au1 128.324(8) 2_655 12_666
Au1 Au2 Au1 98.029(19) 11_656 12_666
Sn5 Au2 Au1 119.348(15) 4_665 3_665
Sn5 Au2 Au1 60.652(14) 7_665 3_665
Y3 Au2 Au1 65.03(5) 3_665 3_665
Y3 Au2 Au1 150.635(15) 2_655 3_665
Y3 Au2 Au1 63.30(5) . 3_665
Au1 Au2 Au1 98.029(19) 2_655 3_665
Au1 Au2 Au1 128.324(8) 11_656 3_665
Au1 Au2 Au1 58.70(3) 12_666 3_665
Sn5 Au2 Au1 119.348(14) 4_665 .
Sn5 Au2 Au1 60.652(14) 7_665 .
Y3 Au2 Au1 150.635(15) 3_665 .
Y3 Au2 Au1 63.30(5) 2_655 .
Y3 Au2 Au1 65.03(5) . .
Au1 Au2 Au1 98.029(19) 2_655 .
Au1 Au2 Au1 128.324(8) 11_656 .
Au1 Au2 Au1 128.324(8) 12_666 .
Au1 Au2 Au1 98.029(19) 3_665 .
Sn5 Au2 Au1 60.652(14) 4_665 10_556
Sn5 Au2 Au1 119.348(14) 7_665 10_556
Y3 Au2 Au1 150.635(15) 3_665 10_556
Y3 Au2 Au1 63.30(5) 2_655 10_556
Y3 Au2 Au1 65.03(5) . 10_556
Au1 Au2 Au1 128.324(8) 2_655 10_556
Au1 Au2 Au1 98.029(19) 11_656 10_556
Au1 Au2 Au1 98.029(19) 12_666 10_556
Au1 Au2 Au1 128.324(8) 3_665 10_556
Au1 Au2 Au1 58.70(3) . 10_556
Au2 Y3 Au1 151.23(3) . 11_666
Au2 Y3 Au1 151.23(3) . 2_665
Au1 Y3 Au1 57.54(5) 11_666 2_665
Au2 Y3 Au1 58.97(5) . 12_666
Au1 Y3 Au1 103.38(6) 11_666 12_666
Au1 Y3 Au1 133.15(9) 2_665 12_666
Au2 Y3 Au1 58.97(5) . 3_665
Au1 Y3 Au1 133.15(9) 11_666 3_665
Au1 Y3 Au1 103.38(6) 2_665 3_665
Au1 Y3 Au1 56.08(5) 12_666 3_665
Au2 Y3 Au1 58.08(5) . .
Au1 Y3 Au1 132.72(9) 11_666 .
Au1 Y3 Au1 103.69(6) 2_665 .
Au1 Y3 Au1 117.05(8) 12_666 .
Au1 Y3 Au1 91.33(5) 3_665 .
Au2 Y3 Au1 58.08(5) . 10_556
Au1 Y3 Au1 103.69(6) 11_666 10_556
Au1 Y3 Au1 132.72(9) 2_665 10_556
Au1 Y3 Au1 91.33(5) 12_666 10_556
Au1 Y3 Au1 117.05(8) 3_665 10_556
Au1 Y3 Au1 54.63(5) . 10_556
Au2 Y3 Au1 87.89(5) . 7_665
Au1 Y3 Au1 120.83(7) 11_666 7_665
Au1 Y3 Au1 63.35(3) 2_665 7_665
Au1 Y3 Au1 118.61(7) 12_666 7_665
Au1 Y3 Au1 62.61(3) 3_665 7_665
Au1 Y3 Au1 59.60(4) . 7_665
Au1 Y3 Au1 114.23(7) 10_556 7_665
Au2 Y3 Au1 87.89(5) . 4_665
Au1 Y3 Au1 63.35(3) 11_666 4_665
Au1 Y3 Au1 120.83(7) 2_665 4_665
Au1 Y3 Au1 62.61(3) 12_666 4_665
Au1 Y3 Au1 118.61(7) 3_665 4_665
Au1 Y3 Au1 114.23(7) . 4_665
Au1 Y3 Au1 59.60(4) 10_556 4_665
Au1 Y3 Au1 173.79(9) 7_665 4_665
Au2 Y3 Sn5 110.17(7) . .
Au1 Y3 Sn5 88.68(7) 11_666 .
Au1 Y3 Sn5 53.61(4) 2_665 .
Au1 Y3 Sn5 167.93(8) 12_666 .
Au1 Y3 Sn5 114.89(3) 3_665 .
Au1 Y3 Sn5 52.45(3) . .
Au1 Y3 Sn5 86.23(7) 10_556 .
Au1 Y3 Sn5 52.58(3) 7_665 .
Au1 Y3 Sn5 125.12(8) 4_665 .
Au2 Y3 Sn5 110.17(7) . 10_556
Au1 Y3 Sn5 53.61(4) 11_666 10_556
Au1 Y3 Sn5 88.68(7) 2_665 10_556
Au1 Y3 Sn5 114.89(3) 12_666 10_556
Au1 Y3 Sn5 167.93(8) 3_665 10_556
Au1 Y3 Sn5 86.23(7) . 10_556
Au1 Y3 Sn5 52.45(3) 10_556 10_556
Au1 Y3 Sn5 125.12(8) 7_665 10_556
Au1 Y3 Sn5 52.58(3) 4_665 10_556
Sn5 Y3 Sn5 72.65(8) . 10_556
Au2 Sn5 Au1 99.92(4) 7_665 3_565
Au2 Sn5 Au1 99.92(4) 7_665 2_665
Au1 Sn5 Au1 117.10(2) 3_565 2_665
Au2 Sn5 Au1 99.92(4) 7_665 .
Au1 Sn5 Au1 117.10(2) 3_565 .
Au1 Sn5 Au1 117.10(2) 2_665 .
Au2 Sn5 Au1 63.22(4) 7_665 9
Au1 Sn5 Au1 67.47(3) 3_565 9
Au1 Sn5 Au1 163.07(7) 2_665 9
Au1 Sn5 Au1 70.09(3) . 9
Au2 Sn5 Au1 63.22(4) 7_665 8_565
Au1 Sn5 Au1 70.09(3) 3_565 8_565
Au1 Sn5 Au1 67.47(3) 2_665 8_565
Au1 Sn5 Au1 163.07(7) . 8_565
Au1 Sn5 Au1 101.27(5) 9 8_565
Au2 Sn5 Au1 63.22(4) 7_665 7_665
Au1 Sn5 Au1 163.07(7) 3_565 7_665
Au1 Sn5 Au1 70.09(3) 2_665 7_665
Au1 Sn5 Au1 67.47(3) . 7_665
Au1 Sn5 Au1 101.27(5) 9 7_665
Au1 Sn5 Au1 101.27(5) 8_565 7_665
Au2 Sn5 Y3 126.32(4) 7_665 2_665
Au1 Sn5 Y3 58.47(5) 3_565 2_665
Au1 Sn5 Y3 61.68(5) 2_665 2_665
Au1 Sn5 Y3 133.72(7) . 2_665
Au1 Sn5 Y3 125.90(5) 9 2_665
Au1 Sn5 Y3 63.20(3) 8_565 2_665
Au1 Sn5 Y3 131.70(5) 7_665 2_665
Au2 Sn5 Y3 126.32(4) 7_665 3_565
Au1 Sn5 Y3 61.68(5) 3_565 3_565
Au1 Sn5 Y3 133.72(7) 2_665 3_565
Au1 Sn5 Y3 58.47(5) . 3_565
Au1 Sn5 Y3 63.20(3) 9 3_565
Au1 Sn5 Y3 131.70(5) 8_565 3_565
Au1 Sn5 Y3 125.90(5) 7_665 3_565
Y3 Sn5 Y3 88.49(6) 2_665 3_565
Au2 Sn5 Y3 126.32(4) 7_665 .
Au1 Sn5 Y3 133.72(7) 3_565 .
Au1 Sn5 Y3 58.47(5) 2_665 .
Au1 Sn5 Y3 61.68(5) . .
Au1 Sn5 Y3 131.70(5) 9 .
Au1 Sn5 Y3 125.90(5) 8_565 .
Au1 Sn5 Y3 63.20(3) 7_665 .
Y3 Sn5 Y3 88.49(6) 2_665 .
Y3 Sn5 Y3 88.49(6) 3_565 .
Au1 Sn6 Au1 180.00(4) . 7
Au1 Sn6 Au1 69.069(14) . 8
Au1 Sn6 Au1 110.931(14) 7 8
Au1 Sn6 Au1 69.069(14) . 9
Au1 Sn6 Au1 110.931(14) 7 9
Au1 Sn6 Au1 110.931(14) 8 9
Au1 Sn6 Au1 110.931(14) . 3
Au1 Sn6 Au1 69.069(14) 7 3
Au1 Sn6 Au1 69.069(14) 8 3
Au1 Sn6 Au1 180.00(4) 9 3
Au1 Sn6 Au1 110.931(14) . 2
Au1 Sn6 Au1 69.069(14) 7 2
Au1 Sn6 Au1 180.00(3) 8 2
Au1 Sn6 Au1 69.069(14) 9 2
Au1 Sn6 Au1 110.931(14) 3 2
Au1 Sn6 Y3 124.77(4) . 9_545
Au1 Sn6 Y3 55.23(4) 7 9_545
Au1 Sn6 Y3 56.71(4) 8 9_545
Au1 Sn6 Y3 119.89(3) 9 9_545
Au1 Sn6 Y3 60.11(3) 3 9_545
Au1 Sn6 Y3 123.29(4) 2 9_545
Au1 Sn6 Y3 55.23(4) . 3_565
Au1 Sn6 Y3 124.77(4) 7 3_565
Au1 Sn6 Y3 123.29(4) 8 3_565
Au1 Sn6 Y3 60.11(3) 9 3_565
Au1 Sn6 Y3 119.89(3) 3 3_565
Au1 Sn6 Y3 56.71(4) 2 3_565
Y3 Sn6 Y3 180.00(9) 9_545 3_565
Au1 Sn6 Y3 56.71(4) . 2_655
Au1 Sn6 Y3 123.29(4) 7 2_655
Au1 Sn6 Y3 60.11(3) 8 2_655
Au1 Sn6 Y3 124.77(4) 9 2_655
Au1 Sn6 Y3 55.23(4) 3 2_655
Au1 Sn6 Y3 119.89(3) 2 2_655
Y3 Sn6 Y3 100.09(4) 9_545 2_655
Y3 Sn6 Y3 79.91(4) 3_565 2_655
Au1 Sn6 Y3 123.29(4) . 8_455
Au1 Sn6 Y3 56.71(4) 7 8_455
Au1 Sn6 Y3 119.89(3) 8 8_455
Au1 Sn6 Y3 55.23(4) 9 8_455
Au1 Sn6 Y3 124.77(4) 3 8_455
Au1 Sn6 Y3 60.11(3) 2 8_455
Y3 Sn6 Y3 79.91(4) 9_545 8_455
Y3 Sn6 Y3 100.09(4) 3_565 8_455
Y3 Sn6 Y3 180.00(9) 2_655 8_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Au1 Sn5 2.8485(9) .
Au1 Sn5 2.8918(12) 7_665
Au1 Au1 2.9032(15) 10_556
Au1 Sn6 2.9073(9) .
Au1 Au2 2.9617(7) .
Au1 Y3 3.016(2) 3_565
Au1 Y3 3.088(2) 2_655
Au1 Y3 3.163(2) .
Au1 Au1 3.1881(17) 7_665
Au1 Y3 3.2502(10) 7_665
Au1 Au1 3.2963(11) 8
Au2 Sn5 2.755(2) 4_665
Au2 Sn5 2.755(2) 7_665
Au2 Y3 2.923(3) 3_665
Au2 Y3 2.923(3) 2_655
Au2 Y3 2.923(3) .
Au2 Au1 2.9617(7) 2_655
Au2 Au1 2.9617(7) 11_656
Au2 Au1 2.9617(7) 12_666
Au2 Au1 2.9617(7) 3_665
Au2 Au1 2.9617(7) 10_556
Y3 Au1 3.016(2) 11_666
Y3 Au1 3.016(2) 2_665
Y3 Au1 3.088(2) 12_666
Y3 Au1 3.088(2) 3_665
Y3 Au1 3.163(2) 10_556
Y3 Au1 3.2502(10) 7_665
Y3 Au1 3.2502(10) 4_665
Y3 Sn5 3.279(2) .
Y3 Sn5 3.279(2) 10_556
Sn5 Au2 2.755(2) 7_665
Sn5 Au1 2.8485(9) 3_565
Sn5 Au1 2.8485(9) 2_665
Sn5 Au1 2.8918(12) 9
Sn5 Au1 2.8918(12) 8_565
Sn5 Au1 2.8918(12) 7_665
Sn5 Y3 3.279(2) 2_665
Sn5 Y3 3.279(2) 3_565
Sn6 Au1 2.9073(9) 7
Sn6 Au1 2.9073(9) 8
Sn6 Au1 2.9073(9) 9
Sn6 Au1 2.9073(9) 3
Sn6 Au1 2.9073(9) 2
Sn6 Y3 3.5006(19) 9_545
Sn6 Y3 3.5006(19) 3_565
Sn6 Y3 3.5006(19) 2_655
Sn6 Y3 3.5006(19) 8_455
